#------------------------------------------------------------------------------
#$Date: 2016-03-23 01:29:41 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179143 $
#$URL: svn://www.crystallography.net/cod/cif/4/31/04/4310442.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4310442
loop_
_publ_author_name
'Philip A. W. Dean'
'Don Craig'
'Ian Dance'
'Vanessa Russell'
'Marcia Scudder'
_publ_section_title
;
 A variable Ag-Cr-oxalate channel lattice:
 [MₓAg~0.5-x~(H₂O)₃]@[Ag~2.5~Cr(C₂O₄)₃], M = K, Cs, Ag
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              443
_journal_page_last               449
_journal_paper_doi               10.1021/ic034988k
_journal_volume                  43
_journal_year                    2004
_chemical_formula_moiety         'C12 Ag5 Cr2 O24 1-,Ag0.14 Cs0.86 1+,6(H2 O)'
_chemical_formula_sum            'C12 H12 Ag5.14 Cr2 Cs0.86 O30'
_chemical_formula_weight         1408.9
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_type_scat_source
'International Tables for X-ray Crystallography, Vol. IV'
_audit_creation_method           'RAELSPUB and manual entry'
_cell_angle_alpha                90
_cell_angle_beta                 113.00(1)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   18.335(6)
_cell_length_b                   14.628(2)
_cell_length_c                   12.383(4)
_cell_measurement_reflns_used    10
_cell_measurement_temperature    294
_cell_measurement_theta_max      13
_cell_measurement_theta_min      12
_cell_volume                     3057.2(15)
_computing_cell_refinement       'CAD4 Version 5.0, 1989'
_computing_data_collection       'CAD4 Version 5.0, 1989'
_computing_data_reduction        'Local program'
_computing_molecular_graphics    'ORTEP-II, (Johnson, 1976)'
_computing_publication_material  'Local programs'
_computing_structure_refinement  'RAELS, (Rae, 1989)'
_computing_structure_solution    'SIR92 (Altomare et al, 1994)'
_diffrn_measurement_device_type  'Nonius CAD-4'
_diffrn_measurement_method       ω--2θ
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.031
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            2827
_diffrn_reflns_theta_max         25
_diffrn_standards_decay_%        5
_diffrn_standards_interval_time  30min
_diffrn_standards_number         1
_exptl_absorpt_coefficient_mu    4.979
_exptl_absorpt_correction_T_max  0.45
_exptl_absorpt_correction_T_min  0.40
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   '(DeMeulenaer & Tompa, 1965)'
_exptl_crystal_colour            purple
_exptl_crystal_density_diffrn    3.06
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             2643.5
_refine_diff_density_max         2.16
_refine_diff_density_min         -1.76
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.92
_refine_ls_hydrogen_treatment    noref
_refine_ls_number_parameters     240
_refine_ls_number_reflns         2441
_refine_ls_R_factor_gt           0.061
_refine_ls_shift/su_max          0.005
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     'w = 1/[σ²(F) + 0.0004F²]'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         0.118
_reflns_number_gt                2441
_reflns_number_total             2689
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            ic034988ksi20030821_071553_5.cif
_cod_data_source_block           5
_cod_original_cell_volume        3057(1)
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               4310442
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 x,y,z
2 x,-y,1/2+z
3 -x,-y,-z
4 -x,y,1/2-z
5 1/2+x,1/2+y,z
6 1/2+x,1/2-y,1/2+z
7 1/2-x,1/2-y,-z
8 1/2-x,1/2+y,1/2-z
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_type_symbol
_atom_site_occupancy
Ag1 0.50000 0.46413(8) 0.75000 0.0462(5) Uani Ag 1.0
Ag2 0.24823(5) 0.19769(5) 0.74440(6) 0.0521(4) Uani Ag 1.0
Ag3 0.07796(6) 0.80991(6) 0.37602(9) 0.0676(5) Uani Ag 1.0
Cr 0.29060(7) 0.49561(8) 0.47630(10) 0.0272(4) Uani Cr 1.0
O1 0.3519(3) 0.4212(4) 0.6135(5) 0.033(1) Uani O 1.0
O2 0.2072(3) 0.4091(4) 0.4655(5) 0.039(1) Uani O 1.0
O3 0.3416(4) 0.3002(5) 0.7169(6) 0.048(2) Uani O 1.0
O4 0.1836(4) 0.2876(4) 0.5593(6) 0.046(2) Uani O 1.0
C1 0.3149(5) 0.3554(5) 0.6332(7) 0.033(2) Uani C 1.0
C2 0.2274(5) 0.3480(6) 0.5457(7) 0.033(2) Uani C 1.0
O5 0.2193(4) 0.5697(4) 0.3436(5) 0.036(1) Uani O 1.0
O6 0.2581(3) 0.5855(4) 0.5672(5) 0.035(1) Uani O 1.0
O7 0.1481(5) 0.6960(4) 0.3055(6) 0.044(2) Uani O 1.0
O8 0.1844(4) 0.7102(4) 0.5452(5) 0.043(2) Uani O 1.0
C3 0.1889(4) 0.6401(6) 0.3713(7) 0.032(2) Uani C 1.0
C4 0.2105(4) 0.6474(5) 0.5060(7) 0.031(2) Uani C 1.0
O9 0.3832(3) 0.5708(4) 0.4895(5) 0.029(1) Uani O 1.0
O10 0.3264(3) 0.4219(4) 0.3720(5) 0.035(1) Uani O 1.0
O11 0.5257(3) 0.4136(4) 0.5863(5) 0.032(1) Uani O 1.0
O12 0.5790(4) 0.5814(5) 0.6989(5) 0.039(1) Uani O 1.0
C5 0.4186(4) 0.5455(5) 0.4244(6) 0.026(2) Uani C 1.0
C6 0.3877(5) 0.4530(5) 0.3587(6) 0.027(2) Uani C 1.0
Cs 0.5088(1) 0.2154(1) 0.8608(2) 0.0710(8) Uani Cs 0.43
Ag' 0.5771(20) 0.1571(23) 0.8034(31) 0.0710(8) Uani Ag 0.03
Ag'' 0.5410(17) 0.2343(18) 0.9383(28) 0.0710(8) Uani Ag 0.04
OW1 -0.0035(6) 0.7058(11) 0.4049(12) 0.127(6) Uani O 1.0
OW2 0.1051(9) 0.4508(16) 0.1642(16) 0.170(9) Uani O 1.0
OW3 0.0610(9) 0.4844(11) -0.0792(23) 0.174(9) Uani O 1.0
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
-1 0 1 0.15
0 0 1 0.14
-1 1 1 0.14
4 -3 -5 0.10
-1 1 0 0.09
1 -1 0 0.09
1 1 0 0.10
-1 -1 0 0.09
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Ag1 O1 152.6(3) 1_555 1_555 4_656 no
O1 Ag1 O11 82.9(2) 1_555 1_555 1_555 no
O1 Ag1 O11 88.6(2) 1_555 1_555 4_656 no
O1 Ag1 O12 123.7(2) 1_555 1_555 1_555 no
O1 Ag1 O12 76.8(2) 1_555 1_555 4_656 no
O1 Ag1 O11 88.6(2) 4_656 1_555 1_555 no
O1 Ag1 O11 82.9(2) 4_656 1_555 4_656 no
O1 Ag1 O12 76.8(2) 4_656 1_555 1_555 no
O1 Ag1 O12 123.7(2) 4_656 1_555 4_656 no
O11 Ag1 O11 143.7(3) 1_555 1_555 4_656 no
O11 Ag1 O12 70.6(2) 1_555 1_555 1_555 no
O11 Ag1 O12 139.8(2) 1_555 1_555 4_656 no
O11 Ag1 O12 139.8(2) 4_656 1_555 1_555 no
O11 Ag1 O12 70.6(2) 4_656 1_555 4_656 no
O12 Ag1 O12 92.5(3) 1_555 1_555 4_656 no
O3 Ag2 O4 69.5(2) 1_555 1_555 1_555 no
O3 Ag2 O6 136.5(2) 1_555 1_555 8_546 no
O3 Ag2 O7 106.2(3) 1_555 1_555 2_565 no
O3 Ag2 O8 90.8(2) 1_555 1_555 8_546 no
O3 Ag2 O10 131.2(2) 1_555 1_555 7_556 no
O4 Ag2 O6 152.0(2) 1_555 1_555 8_546 no
O4 Ag2 O7 79.9(2) 1_555 1_555 2_565 no
O4 Ag2 O8 143.9(2) 1_555 1_555 8_546 no
O4 Ag2 O10 82.8(2) 1_555 1_555 7_556 no
O6 Ag2 O7 81.7(2) 8_546 1_555 2_565 no
O6 Ag2 O8 48.5(2) 8_546 1_555 8_546 no
O6 Ag2 O10 82.8(2) 8_546 1_555 7_556 no
O7 Ag2 O8 76.9(2) 2_565 1_555 8_546 no
O7 Ag2 O10 107.5(2) 2_565 1_555 7_556 no
O8 Ag2 O10 130.6(2) 8_546 1_555 7_556 no
O7 Ag3 O8 65.5(2) 1_555 1_555 1_555 no
O7 Ag3 O9 134.9(2) 1_555 1_555 7_566 no
O7 Ag3 O12 86.6(2) 1_555 1_555 6_464 no
O7 Ag3 OW1 94.0(5) 1_555 1_555 1_555 no
O8 Ag3 O9 85.6(2) 1_555 1_555 7_566 no
O8 Ag3 O12 136.1(2) 1_555 1_555 6_464 no
O8 Ag3 OW1 80.4(3) 1_555 1_555 1_555 no
O9 Ag3 O12 92.4(2) 7_566 1_555 6_464 no
O9 Ag3 OW1 115.4(5) 7_566 1_555 1_555 no
O12 Ag3 OW1 137.5(3) 6_464 1_555 1_555 no
O1 Cr O2 82.4(2) 1_555 1_555 1_555 no
O1 Cr O5 173.9(3) 1_555 1_555 1_555 no
O1 Cr O6 94.3(2) 1_555 1_555 1_555 no
O1 Cr O9 93.1(2) 1_555 1_555 1_555 no
O1 Cr O10 92.2(2) 1_555 1_555 1_555 no
O2 Cr O5 93.0(3) 1_555 1_555 1_555 no
O2 Cr O6 93.9(3) 1_555 1_555 1_555 no
O2 Cr O9 173.3(3) 1_555 1_555 1_555 no
O2 Cr O10 93.1(3) 1_555 1_555 1_555 no
O5 Cr O6 81.9(2) 1_555 1_555 1_555 no
O5 Cr O9 91.8(3) 1_555 1_555 1_555 no
O5 Cr O10 92.1(2) 1_555 1_555 1_555 no
O6 Cr O9 91.3(2) 1_555 1_555 1_555 no
O6 Cr O10 171.1(2) 1_555 1_555 1_555 no
O9 Cr O10 82.2(2) 1_555 1_555 1_555 no
Ag1 O1 Cr 121.2(3) 1_555 1_555 1_555 no
Ag1 O1 C1 123.7(5) 1_555 1_555 1_555 no
Cr O1 C1 115.1(5) 1_555 1_555 1_555 no
Cr O2 C2 114.8(5) 1_555 1_555 1_555 no
Cr O2 Ag' 138.1(9) 1_555 1_555 6_454 no
C2 O2 Ag' 103.7(9) 1_555 1_555 6_454 no
Ag2 O3 C1 116.8(6) 1_555 1_555 1_555 no
Ag2 O3 Cs 105.4(2) 1_555 1_555 1_555 no
Ag2 O3 Ag' 88.8(8) 1_555 1_555 4_656 no
C1 O3 Cs 134.7(6) 1_555 1_555 1_555 no
C1 O3 Ag' 119.0(10) 1_555 1_555 4_656 no
Ag2 O4 C2 113.4(6) 1_555 1_555 1_555 no
Ag2 O4 Cs 132.3(2) 1_555 1_555 6_454 no
Ag2 O4 Ag'' 119.8(8) 1_555 1_555 6_454 no
C2 O4 Cs 114.3(5) 1_555 1_555 6_454 no
C2 O4 Ag'' 126.3(9) 1_555 1_555 6_454 no
O1 C1 O3 126.1(7) 1_555 1_555 1_555 no
O1 C1 C2 114.1(7) 1_555 1_555 1_555 no
O3 C1 C2 119.8(7) 1_555 1_555 1_555 no
O2 C2 O4 126.4(8) 1_555 1_555 1_555 no
O2 C2 C1 113.7(6) 1_555 1_555 1_555 no
O4 C2 C1 119.9(8) 1_555 1_555 1_555 no
Cr O5 C3 115.7(5) 1_555 1_555 1_555 no
Ag2 O6 Cr 163.1(3) 8_556 1_555 1_555 no
Ag2 O6 C4 80.9(4) 8_556 1_555 1_555 no
Cr O6 C4 115.0(5) 1_555 1_555 1_555 no
Ag2 O7 Ag3 102.4(2) 2_564 1_555 1_555 no
Ag2 O7 C3 105.7(6) 2_564 1_555 1_555 no
Ag3 O7 C3 119.8(6) 1_555 1_555 1_555 no
Ag2 O8 Ag3 142.8(3) 8_556 1_555 1_555 no
Ag2 O8 C4 104.9(5) 8_556 1_555 1_555 no
Ag3 O8 C4 112.3(5) 1_555 1_555 1_555 no
O5 C3 O7 126.3(8) 1_555 1_555 1_555 no
O5 C3 C4 112.8(7) 1_555 1_555 1_555 no
O7 C3 C4 120.9(8) 1_555 1_555 1_555 no
O6 C4 O8 125.4(8) 1_555 1_555 1_555 no
O6 C4 C3 114.4(7) 1_555 1_555 1_555 no
O8 C4 C3 120.1(7) 1_555 1_555 1_555 no
Ag3 O9 Cr 119.3(2) 7_566 1_555 1_555 no
Ag3 O9 C5 125.7(5) 7_566 1_555 1_555 no
Cr O9 C5 114.9(5) 1_555 1_555 1_555 no
Ag2 O10 Cr 123.0(3) 7_556 1_555 1_555 no
Ag2 O10 C6 121.3(5) 7_556 1_555 1_555 no
Cr O10 C6 114.9(5) 1_555 1_555 1_555 no
Ag1 O11 C5 112.9(5) 1_555 1_555 3_666 no
Ag1 O11 Cs 89.2(2) 1_555 1_555 4_656 no
Ag1 O11 Ag'' 99.1(6) 1_555 1_555 4_656 no
C5 O11 Cs 136.4(5) 3_666 1_555 4_656 no
C5 O11 Ag'' 140.4(8) 3_666 1_555 4_656 no
Ag1 O12 Ag3 90.6(2) 1_555 1_555 6_565 no
Ag1 O12 C6 109.9(5) 1_555 1_555 3_666 no
Ag3 O12 C6 151.8(5) 6_565 1_555 3_666 no
O9 C5 O11 125.1(7) 1_555 1_555 3_666 no
O9 C5 C6 114.2(6) 1_555 1_555 1_555 no
O11 C5 C6 120.6(7) 3_666 1_555 1_555 no
O10 C6 O12 126.5(7) 1_555 1_555 3_666 no
O10 C6 C5 113.5(6) 1_555 1_555 1_555 no
O12 C6 C5 120.0(7) 3_666 1_555 1_555 no
O3 Cs O4 155.3(2) 1_555 1_555 6_555 no
O3 Cs O11 60.9(2) 1_555 1_555 4_656 no
O3 Cs OW1 100.2(3) 1_555 1_555 8_546 no
O3 Cs OW2 77.6(4) 1_555 1_555 7_556 no
O4 Cs O11 94.4(2) 6_555 1_555 4_656 no
O4 Cs OW1 69.5(2) 6_555 1_555 8_546 no
O4 Cs OW2 119.7(4) 6_555 1_555 7_556 no
O11 Cs OW1 75.4(3) 4_656 1_555 8_546 no
O11 Cs OW2 124.3(3) 4_656 1_555 7_556 no
OW1 Cs OW2 77.5(4) 8_546 1_555 7_556 no
O2 Ag' O3 89.3(10) 6_555 1_555 4_656 no
O2 Ag' OW2 85.7(11) 6_555 1_555 6_555 no
O2 Ag' OW3 63.2(8) 6_555 1_555 5_546 no
O3 Ag' OW2 99.1(14) 4_656 1_555 6_555 no
O3 Ag' OW3 152.2(13) 4_656 1_555 5_546 no
OW2 Ag' OW3 83.6(11) 6_555 1_555 5_546 no
O4 Ag'' O11 119.4(11) 6_555 1_555 4_656 no
O4 Ag'' OW1 93.3(11) 6_555 1_555 8_546 no
O11 Ag'' OW1 90.0(10) 4_656 1_555 8_546 no
Ag3 OW1 Cs 113.7(7) 1_555 1_555 8_556 no
Ag3 OW1 Ag'' 116.0(9) 1_555 1_555 8_556 no
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ag1 O1 2.653(5) 1_555 1_555 no
Ag1 O1 2.653(5) 1_555 4_656 no
Ag1 O11 2.371(5) 1_555 1_555 no
Ag1 O11 2.371(5) 1_555 4_656 no
Ag1 O12 2.481(6) 1_555 1_555 no
Ag1 O12 2.481(6) 1_555 4_656 no
Ag2 O3 2.398(6) 1_555 1_555 no
Ag2 O4 2.503(6) 1_555 1_555 no
Ag2 O6 2.892(6) 1_555 8_546 no
Ag2 O7 2.729(8) 1_555 2_565 no
Ag2 O8 2.415(6) 1_555 8_546 no
Ag2 O10 2.338(5) 1_555 7_556 no
Ag3 O7 2.463(7) 1_555 1_555 no
Ag3 O8 2.670(7) 1_555 1_555 no
Ag3 O9 2.323(5) 1_555 7_566 no
Ag3 O12 2.714(6) 1_555 6_464 no
Ag3 OW1 2.257(12) 1_555 1_555 no
Cr O1 1.961(6) 1_555 1_555 no
Cr O2 1.949(6) 1_555 1_555 no
Cr O5 1.976(6) 1_555 1_555 no
Cr O6 1.968(6) 1_555 1_555 no
Cr O9 1.976(5) 1_555 1_555 no
Cr O10 1.982(6) 1_555 1_555 no
O1 C1 1.255(10) 1_555 1_555 no
O2 C2 1.278(11) 1_555 1_555 no
O2 Ag' 2.630(32) 1_555 6_454 no
O3 C1 1.253(11) 1_555 1_555 no
O3 Cs 3.138(8) 1_555 1_555 no
O3 Ag' 2.638(35) 1_555 4_656 no
O4 C2 1.249(10) 1_555 1_555 no
O4 Cs 3.188(7) 1_555 6_454 no
O4 Ag'' 2.475(29) 1_555 6_454 no
C1 C2 1.550(11) 1_555 1_555 no
O5 C3 1.280(11) 1_555 1_555 no
O6 Ag2 2.892(6) 1_555 8_556 no
O6 C4 1.281(10) 1_555 1_555 no
O7 Ag2 2.729(8) 1_555 2_564 no
O7 C3 1.191(10) 1_555 1_555 no
O8 Ag2 2.415(6) 1_555 8_556 no
O8 C4 1.220(10) 1_555 1_555 no
C3 C4 1.560(12) 1_555 1_555 no
O9 Ag3 2.323(5) 1_555 7_566 no
O9 C5 1.271(9) 1_555 1_555 no
O10 Ag2 2.338(5) 1_555 7_556 no
O10 C6 1.281(9) 1_555 1_555 no
O11 C5 1.234(9) 1_555 3_666 no
O11 Cs 3.092(6) 1_555 4_656 no
O11 Ag'' 2.859(26) 1_555 4_656 no
O12 Ag3 2.714(6) 1_555 6_565 no
O12 C6 1.216(10) 1_555 3_666 no
C5 O11 1.234(9) 1_555 3_666 no
C5 C6 1.567(10) 1_555 1_555 no
C6 O12 1.216(10) 1_555 3_666 no
Cs O4 3.188(7) 1_555 6_555 no
Cs O11 3.092(6) 1_555 4_656 no
Cs OW1 2.945(15) 1_555 8_546 no
Cs OW2 3.141(22) 1_555 7_556 no
Ag' O2 2.630(32) 1_555 6_555 no
Ag' O3 2.638(35) 1_555 4_656 no
Ag' OW2 2.533(44) 1_555 6_555 no
Ag' OW3 2.987(40) 1_555 5_546 no
Ag'' O4 2.475(29) 1_555 6_555 no
Ag'' O11 2.859(26) 1_555 4_656 no
Ag'' OW1 2.338(35) 1_555 8_546 no
OW1 Cs 2.945(15) 1_555 8_556 no
OW1 Ag'' 2.338(35) 1_555 8_556 no
OW2 Cs 3.141(22) 1_555 7_556 no
OW2 Ag' 2.533(44) 1_555 6_454 no
OW3 Ag' 2.987(40) 1_555 5_454 no
